- Solid oxide fuel cell
A solid oxide fuel cell (SOFC) is an electrochemical conversion device that produces electricity directly from oxidizing a fuel. Fuel cells are characterized by their electrolyte material and, as the name implies, the SOFC has a solid oxide, or
ceramic, electrolyte. Advantages of this class of fuel cells include high efficiencies, long term stability, fuel flexibility, low emissions, and cost. The largest disadvantage is the high operating temperature which results in longer start up times and mechanical/chemical compatibility issues.
Solid oxide fuel cells have a wide variety of applications from use as auxiliary power units in vehicles to stationary power generation with outputs from 100 W to 2 MW. They operate at very high temperatures, typically between 500 and 1,000°C. Typical values for efficiency of a single SOFC device is around 60 plus percent. However, the byproduct gases can be used to fire a secondary
gas turbineto improve electrical efficiency. This enables efficiency to reach as much as 85% in these hybrid systems, called combined heat and power(CHP) device. In these cells, it is most common to have oxygenions diffusing through a solid oxide electrolytematerial at high temperature to react with hydrogenon the anodeside.
Due to the high operating temperature of SOFCs, they have no need for expensive catalyst, which is the case of proton-exchange fuel cells (
platinum) and most other types of low temperature fuel cells. Because of these high temperatures, fuels can be internally reformed within the anode unlike in PEMFCs where catalyst poisoningby carbon monoxidewill occur. This allows SOFCs to operate on a wide variety of different fuels such as methane, propane, butane, natural gas, fermentation gas, gasified biomassand paint fumes. However, sulfurcomponents present in the fuel must be removed before entering the cell, but this can easily be done by an activated carbonbed or a zincabsorbent. SOFCs can increase efficiency by using the heat given off by the exothermic electrochemical oxidation of hydrogen for endothermic reforming process. Internal reforming also leads to a large decrease in the balance of plant costs in designing a full system
Thermal expansion demands a uniform and slow heating process at startup. Typically, 8 hours or more are to be expected. Micro-tubular geometries promise much faster start up times, typically on the order of minutes.ref|research
Unlike most other types of
fuel cells, SOFCs can have multiple geometries. The planar geometry is the typical sandwich type geometry employed by most types of fuel cells, where the electrolyte is sandwiched in between the electrodes. SOFCs can also be made in tubular geometries where either air or fuel is passed through the inside of the tube and the other gas is passed along the outside of the tube. The tubular design is advantageous because it is much easier to seal air from the fuel. The performance of the planar design is currently better than the performance of the tubular design however, because the planar design has a lower resistance comparatively. Other geometries of SOFCs include modified planar cells (MPC or MPSOFC), where a wave-like structure replaces the traditional flat configuration of the planar cell. Such designs are highly promising, because they share the advantages of both planar cells (low resistance) and tubular cells (easier sealing).ref|research
A solid oxide fuel cell is made up of four layers, three of which are
ceramics (hence the name). A single cell consisting of these four layers stacked together is typically only a few millimeters thick. Hundreds of these cells are then connected in series to form what most people refer to as an “SOFC stack.” The ceramics used in SOFCs do not become electrically and ionically active until they reach very high temperature and as a consequence the stacks have to run at temperatures ranging from 600 to 1,000 °C. Reduction of oxygen into oxygen ions occurs at the cathode. These ions can then diffuse through the solid oxide electrolyte to the anode where they can electrochemically oxidize the fuel. In this reaction, a water byproduct is given off as well as two electrons. These electrons then flow through an external circuit where they can do work. The cycle then repeats as those electrons enter the cathode material again.
The ceramic [anode] layer must be very porous to allow the fuel to flow towards the electrolyte. Like the cathode, it must conduct electrons, with ionic conductivity a definite asset. The most common material used is a
cermetmade up of nickelmixed with the ceramic material that is used for the electrolyte in that particular cell, typically YSZ (yttria stabilized zirconia). The anode is commonly the thickest and strongest layer in each individual cell, because is has the smallest polarization losses, and is often the layer that provides the mechanical support. Electrochemically speaking, the anode’s job is to use the oxygen ions that diffuse through the electrolyte to oxidize the hydrogen fuel. The
oxidation reaction between the oxygen ions and the hydrogen produces both water and electricity.
The electrolyte is a dense layer of oxygen ion conducting ceramic. Its electronic conductivity must be kept as low as possible to prevent losses from leakage currents. The high operating temperatures of SOFCs allow the kinetics of oxygen ion transport to be sufficient for good performance. However, as the operating temperature approaches the lower limit for SOFCs at around 600°C, the electrolyte begins to have large ionic transport resistances and affect the performance. Popular electrolyte materials include yttrium stabilized zirconia (
YSZ) (often the 8% form Y8SZ) and gadolinium doped ceria (GDC).
cathode, or air electrode, is a thin porous layer on the electrolyte where oxygen reduction takes place. The overall reaction is written in Kröger-Vink Notationas follows:
Cathode materials must be, at minimum, electronically conductive. Currently,
lanthanum strontium manganite(LSM) is the cathode material of choice for commercial use because of its compatibility with doped zirconia electrolytes. Mechanically, it has similar coefficient of thermal expansion to YSZ and thus limits stresses built up because of CTE mismatch. Also, LSM has low levels of chemical reactivity with YSZ which extends the lifetime of the material. Unfortunately, LSM is a poor ionic conductor, and so the electrochemically active reaction is limited to the triple phase boundary (TPB) where the electrolyte, air and electrode meet. LSM works well as a cathode at high temperatures, but its performance quickly falls as the operating temperature is lowered below 800°C. In order to increase the reaction zone beyond the TPB, a potential cathode material must be able to conduct both electrons and oxygen ions. Composite cathodes consisting of LSM YSZ have been used to increase this triple phase boundary length. Mixed ionic/electronic conducting (MIEC) ceramics, such as the perovskite LSCF, are also being researched for use in intermediate temperature SOFCs as they are more active and can makeup for the increase in the activation energy of reaction.
The interconnect can be either a metallic or ceramic layer that sits between each individual cell. Its purpose is to connect each cell in series, so that the electricity each cell generates can be combined. Because the interconnect is exposed to both the oxidizing and reducing side of the cell at high temperatures, it must be extremely stable. For this reason, ceramics have been more successful in the long term than metals as interconnect materials. However, these ceramic interconnect materials are very expensive as compared to metals. Nickel- and steel-based alloys are becoming more promising as lower temperature (600-800°C) SOFCs are developed. The most common intermetallic materials used today are doped lanthanum chromites. Ceramic-metal composites called 'cermet' are also under consideration, as they have demonstrated thermal stability at high temperatures and excellent electrical conductivity.
Polarizations, or overpotentials, are losses in voltage due to imperfections in materials, microstructure, and design of the fuel cell. Polarizations result from ohmic resistance of oxygen ions conducting through the electrolyte (iRΩ), electrochemical activation barriers at the anode and cathode, and finally concentration polarizations due to inability of gases to diffuse at high rates through the porous anode and cathode (shown as ηA for the anode and ηC for cathode).ref|research
In SOFCs, it is typically most important to focus on the ohmic and concentration polarizations since high operating temperatures experience little activation polarization. However, as the lower limit of SOFC operating temperature is approached (~600°C), these polarizations do become important.3
Ohmic losses in an SOFC result from ionic conductivity through the electrolyte. This is inherently a materials property of the crystal structure and atoms involved. However, to maximize the ionic conductivity, several methods can be done. Firstly, operating at higher temperatures can significantly decrease these ohmic losses. Also, substitutional doping methods to further finetune the crystal structure and control defect concentrations can also play a significant role in increasing the conductivity. Another way to decrease ohmic resistance is to decrease the thickness of the electrolyte layer.6
The concentration polarization is the result of the finite gas diffusion processes that govern movement of the gases into and out of the electrochemical reaction. The rate of mass transport of gases is described by Fick’s first law. Therefore the maximum rate of gas diffusion (which is directly related to the maximum current density that can be obtained) is found when the concentration of fuel at the electrochemically active area is assumed to be zero. The potential difference between operation where current is flowing and not flowing is the concentration polarization and is equal to:
* = gas constant
* = operating temperature
* = number of electrons exchanged in electrochemical reaction
* = Faraday's constant
* = operating current
* = max current
The concentration polarization is highly dependent on the gases used as well as the distance that they must diffuse through. Pore volume percentage as well as diffusion length can be varied to optimize these properties. For similar geometries, cathode concentrations are much larger than anode concentrations due to the lower diffusivities of O2/N2 in the cathode than H2/H2O in the anode.
The activation polarization is the result of the kinetics involved with the electrochemical reactions. Each reaction has a certain activation barrier that must be overcome in order to proceed and this barrier leads to the polarization. The activation barrier is the result of many complex electrochemical reaction steps where typically the rate limiting step is responsible for the polarization. The polarization equation shown below is found by solving the Butler-Volmer equation in the high current density regime (where the cell typically operates)
* = gas constant
* = operating temperature
* = electron transfer coefficient
* = electrons associated with the electrochemical reaction
* = Faraday's constant
* = operating current
* = exchange current density
The polarization can be modified most easily by microstructural optimization. The Triple Phase Boundary (TPB) length, which is the length where porous, ionic and electronically conducting pathways all meet, directly relates to the electrochemically active length in the cell. The larger the length, the more reactions can occur and thus the less the activation polarization. Optimization of TPB length can be done by processing conditions to affect mircrostructure or by materials selection to use a mixed ionic/electronic conductor to further increase TPB length.
Research is going now in the direction of lower-temperature SOFC (600°C) in order to decrease the materials cost, which will enable the use of metallic materials with better mechanical properties and
Research is currently underway to improve the fuel flexibility of SOFCs. While stable operation has been achieved on a variety of hydrocarbon fuels, these cells typically rely on external fuel processing. For the case of
natural gas, the fuel is either externally or internally reformed and the sulfurcompounds are removed. These processes add to the cost and complexity of SOFC systems. Work is underway at a number of institutions to improve the stability of anode materials for hydrocarbon oxidation and, therefore, relax the requirements for fuel processing and decrease SOFC balance of plant costs.
Research is also going on in reducing start-up time to be able to implement SOFCs in mobile applications. Due to their fuel flexibility they may run on partially reformed
diesel, and this makes SOFCs interesting as auxiliary power units (APU) in refrigerated trucks.
Specifically, Delphi Automotive Systems and
BMWare developing an SOFC that will power auxiliary units in automobiles. A high-temperature SOFC will generate all of the needed electricity to allow the engine to be smaller and more efficient. The SOFC would run on the same gasolineor diesel as the engine and would keep the air conditioning unit and other necessary electrical systems running while the engine shuts off when not needed (e.g., at a stop light).
Rolls-Royce is developing solid-oxide fuel cells produced by
screen printingonto inexpensive ceramic materials. Rolls-Royce Fuel Cell Systems Ltd is developing a SOFC gas turbine hybrid system fueled by natural gas for power generation applications on the order of a megawatt.ref|research
Ceres Power Ltd. has developed a low cost and low temperature (500-600 degrees) SOFC stack using cerium gadolinium oxide (CGO) in place of current industry standard ceramic,
yttriastabilized zirconia( YSZ), which allows the use of stainless steelto support the ceramic.
Solid Cell Inc. has developed a unique, low cost cell architecture that combines properties of planar and tubular designs, along with a Cr-free
Advanced fuel cell research at institutes of higher learning is becoming more and more popular. The high temperature electrochemistry center (HITEC) at the University of Florida, Gainesville, led by Dr. E.D. Wachsman, is focused on studying ionic transport, electrocatalytic phenomena and microstructural characterization of ion conducting materials.
SOFCs that operate in an intermediate temperature (IT) range, meaning between 600 and 800°C, are named ITSOFCs. Because of the high degradation rates and materials costs incurred at temperatures in excess of 900°C, it is economically more favorable to operate SOFCs at lower temperatures. The push for high performance ITSOFCs is currently the topic of much research and development. One area of focus is the cathode material. It is thought that the oxygen reduction reaction is responsible for much of the loss in performance so the catalytic activity of the cathode is being studied and enhanced through various techniques, including catalyst impregnation.
Auxiliary power unit
Glossary of fuel cell terms
Notes and references
#cite journal | author=Sharke, Paul | title=Freedom of Choice | journal=Mechanical Engineering | volume=126 | issue=10 | year=2004 | pages=33
#cite journal | author=Adamson, F | title=Propagating Reaction Fronts in Zirconia Tubes | journal=PhD thesis | year=2004
#cite journal | author=Singhal, S., Kendall, K. | title=High Temperature Solid Oxide Fuel Cells | journal= | year=2003
* [http://www.fuelcells.bham.ac.uk University of Birmingham Fuel Cell Group]
* [http://www.azom.com/details.asp?ArticleID=919&head=Solid+Oxide+Fuel+Cells Azom.com article on SOFCs]
*cite web | title=Development of SOFC Technology | url=http://www.msrihome.com/FuelCell.html Materials & Systems Research, Inc.'s (MSRI) | work=www.msrihome.com
* [http://www.csa.com/discoveryguides/fuecel/overview.php CSA Overview of SOFCs]
* [http://www.fossil.energy.gov/programs/powersystems/fuelcells/fuelcells_solidoxide.html US Deptartment of Energy page on SOFCs]
* [http://www.iit.edu/~smart/garrear/fuelcells.htm Illinois Institute of Technology page on SOFCs] url=http://www.prototech.no/tekstsider.cfm?artid=6559 | accessdate = 2006-03-03
* [http://www.technologyreview.com/read_article.aspx?ch=biztech&sc=&id=16965&pg=1 More Powerful Fuel Cells Get Closer To Market] - a significant step in making high-temperature fuel cells practical.
* [http://hitec.mse.ufl.edu/ Website for the High Temperature Electro-chemistry Center]
* [http://www.solidcell.net/ Solid Cell Inc. - SOFC Developer]
* [http://glassproperties.com/sofc/ SOFC glass-ceramic sealing]
* [http://www.ecw.org/prod/207-R.pdf Assessment of Solid Oxide Fuel Cells in Building Applications Phase 1: Modeling and Preliminary Analyses]
Wikimedia Foundation. 2010.
Look at other dictionaries:
Solid Oxide Fuel Cell — Tubulare SOFC von Siemens Powergeneration Die Festoxidbrennstoffzelle (engl. Solid Oxide Fuel Cell, SOFC) ist eine Hochtemperatur Brennstoffzelle, die bei einer Betriebstemperatur von 650–1000 °C betrieben wird. Der Elektrolyt dieses Zelltyps… … Deutsch Wikipedia
Fuel cell — For other uses, see Fuel cell (disambiguation). Demonstration model of a direct methanol fuel cell. The actual fuel cell stack is the layered cube shape in the center of the image A fuel cell is a device that converts the chemical energy from a… … Wikipedia
fuel cell — a device that produces a continuous electric current directly from the oxidation of a fuel, as that of hydrogen by oxygen. [1920 25] * * * Device that converts chemical energy of a fuel directly into electricity (see electrochemistry). Fuel cells … Universalium
Direct carbon fuel cell — A Direct Carbon Fuel Cell (DCFC) is a fuel cell that uses a carbon rich material as a fuel. The cell produces energy by combining carbon and oxygen, which releases carbon dioxide as a by product. The total reaction of the cell is C + O2 → CO2.… … Wikipedia
Protonic ceramic fuel cell — The Protonic ceramic fuel cell or PCFC is a fuel cell based on a ceramic electrolyte material that exhibits high protonic conductivity at elevated temperatures. PCFCs share the thermal and kinetic advantages of high temperature operation at 700… … Wikipedia
Molten carbonate fuel cell — Scheme of a molten carbonate fuel cell Molten carbonate fuel cells (MCFCs) are high temperature fuel cells, that operate at temperatures of 600°C and above. Molten carbonate fuel cells (MCFCs) are currently being developed for natural gas, biogas … Wikipedia
Direct methanol fuel cell — Direct methanol fuel cells or DMFCs are a subcategory of proton exchange fuel cells in which methanol is used as the fuel. Their main advantage is the ease of transport of methanol, an energy dense yet reasonably stable liquid at all… … Wikipedia
Electro-galvanic fuel cell — 3 electro galvanic fuel cells from a rebreather An electro galvanic fuel cell is an electrical device, one form of which is commonly used to measure the concentration of oxygen gas in scuba diving and medical equipment. A chemical reaction occurs … Wikipedia
Formic acid fuel cell — Direct formic acid fuel cells or DFAFCs are a subcategory of proton exchange membrane fuel cells where, the fuel, formic acid, is not reformed, but fed directly to the fuel cell. Their applications include small, portable electronics such as… … Wikipedia
Direct-ethanol fuel cell — Direct ethanol fuel cells or DEFCs are a subcategory of Proton exchange fuel cells where the fuel, ethanol, is fed directly to the fuel cell. Contents 1 Advantages 2 Reaction 3 Issues 4 … Wikipedia